INSTITUTE OF PHYSICS PUBLISHING
MEASUREMENT SCIENCE AND TECHNOLOGY
Meas. Sci. Technol. 14 (2003) R49–R61
Optical fibre long-period grating sensors: characteristics and application Stephen W James and Ralph P Tatam Optical Sensors Group, Centre for Photonics and Optical Engineering, School of Engineering, Cranfield University, Cranfield, Bedford MK43 OAL, UK E-mail: [email protected]
Received 24 October 2002, accepted for publication 13 November 2002 Published 26 March 2003 Online at stacks.iop.org/MST/14/R49 Abstract Recent research on fibre optic long-period gratings (LPGs) is reviewed with emphasis placed upon the characteristics of LPGs that make them attractive for applications in sensing strain, temperature, bend radius and external index of refraction. The prospect of the development of multi-parameter sensors, capable of simultaneously monitoring a number of these measurands will be discussed. Keywords: fibre optics, fibre sensors, fibre gratings, long period gratings,
strain, temperature, bend sensor, refractive index (Some figures in this article are in colour only in the electronic version)
1. Introduction The development of fibre gratings has had a significant impact on research and development in telecommunications and fibre optic sensing. Fibre gratings are intrinsic devices that allow control over the properties of light propagating within the fibre—they are used as spectral filters, as dispersion compensating components and in wavelength division multiplexing systems. The sensitivity of their properties to perturbation of the fibre by the surrounding environmental conditions has led to extensive study of their use as fibre sensor elements. Fibre gratings consist of a periodic perturbation of the properties of the optical fibre, generally of the refractive index of the core, and fall into two general classifications based upon the period of the grating. Short-period fibre gratings, or fibre Bragg gratings (FBGs), have a sub-micron period and act to couple light from the forward-propagating mode of the optical fibre to a backward, counterpropagating mode . This coupling occurs at a specific wavelength, defined by the Bragg condition for the fibre grating, with the FBG acting as a narrowband reflection filter and as a narrow-band channel-dropping filter when operated in transmission. The Bragg wavelength is governed by the period of the FBG and the effective index
of the propagating mode, with the result that a change in either of these parameters, induced for example by a change in temperature or strain, changes the wavelength, forming the basis of the many reported FBG sensing schemes. Typically, FBGs deployed as sensors have lengths of the order of 5 mm, with sensitivities to temperature and strain of 13 pm K −1 and 1 pm µε −1 respectively, for FBGs operating at 1300 nm . The long-period grating (LPG) has a period typically in the range 100 µm to 1 mm, as illustrated in figure 1. The LPG promotes coupling between the propagating core mode and co-propagating cladding modes. The high attenuation of the cladding modes results in the transmission spectrum of the fibre containing a series of attenuation bands centred at discrete wavelengths, each attenuation band corresponding to the coupling to a different cladding mode. Examples of the transmission spectra of LPGs are shown in figure 2. The exact form of the spectrum, and the centre wavelengths of the attenuation bands, are sensitive to the period of the LPG, the length of the LPG (typically of the order of 30 mm) and to the local environment: temperature, strain, bend radius and to the refractive index of the medium surrounding the fibre . Changes in these parameters can modify the period of the LPG and/or the differential refractive index of the core and cladding modes. This then modifies the phase matching conditions for
0957-0233/03/050049+13$30.00 © 2003 IOP Publishing Ltd Printed in the UK
Figure 1. Schematic of an LPG.
80 70 60 50 40 30 20 10
coupling to the cladding modes, and results in a change in the central wavelengths of the attenuation bands. The sensitivity to a particular measurand is dependent upon the composition of the fibre and upon the order of the cladding mode to which the guided optical power is coupled, and is thus different for each attenuation band. This range of responses makes them particularly attractive for sensor applications, with the prospect for multi-parameter sensing using a single sensor element . This review will discuss the properties of LPGs and the methods employed in their fabrication. This will be followed by an examination of the theoretical background of LPGs, a discussion of their sensitivities to a range of measurands with a review of their implementation as sensor elements and a discussion of current trends in LPG sensor research.
2. LPG fabrication The fabrication of LPGs relies upon the introduction of a periodic modulation of the optical properties of the fibre. This may be achieved by permanent modification of the refractive index of the core of the optical fibre or by physical deformation of the fibre. The modulation of the core refractive index has been achieved by ultraviolet (UV) irradiation [4–7], ion implantation , irradiation by femtosecond pulses in the infrared , irradiation by CO2 lasers [10, 11], diffusion of dopants into the core [12, 13], relaxation of mechanical stress  and electrical discharges [15, 16]. The deformation of the fibre has been achieved mechanically [17, 18], by tapering the fibre  or by deformation of the core [20, 21] or cladding . LPGs have been fabricated in photonic crystal fibre by periodically collapsing the holes of the fibre using CO2 laser heat treatment . The UV-induced index modulation is typically achieved in Ge-doped silica fibres using wavelengths between 193 and 266 nm . This is the most widely utilized method for the fabrication of LPGs. The refractive index change is associated with the formation of Ge-related glass defects. Fibres with high photosensitivity have been developed by co-doping the core with boron and germanium  and by hydrogen loading . The refractive index modulation may be built up on a point by point basis—a very flexible technique—or the entire length of the LPG may be formed simultaneously by exposure of the fibre though an amplitude mask , via a patterned mirror  or using a microlens array —facilitating rapid and reproducible LPG fabrication. A typical LPG fabrication configuration, using UV irradiation through an amplitude mask, is shown in figure 3. The output from a UV laser source is used to illuminate the R50
950 1000 1050 1100
Figure 2. Transmission spectrum of (a) an LPG of length 40 mm and period 400 µm, fabricated in B–Ge co-doped photosensitive optical fibre with a cut-off wavelength of 644 nm (after ). (b) An LPG fabricated in Corning SMF-28 with period 320 µm (after ). spectrometer
V groove amplitude mask
optical fibre UV laser
broadband optical source
Figure 3. LPG fabrication using a UV laser.
optical fibre through an amplitude mask of appropriate period, which may be fabricated in chrome-plated silica  or from a metal foil, for example by milling a copper foil using a Cu vapour laser . The cylindrical lens produces a line focus oriented parallel to the axis of the fibre.
The use of UV exposure is well established, due to its widespread use in the fabrication of FBGs . Its use has implications for the spectral characteristics and stability of the LPG spectrum. UV exposure of optical fibres is known to induce birefringence, which can produce a polarization splitting in the attenuation bands for LPGs fabricated in nonpolarization-maintaining fibres . The refractive index change is known to contain an unstable component, which decays in time causing a significant change in the central wavelengths of the attenuation bands and in the coupling strength . This unstable component may be removed by thermal annealing, but needs to be taken into account when designing an LPG for a particular application. The use of hydrogen loading of fibres to enhance their photosensitivity can result in further changes to the central wavelength and peak loss of the attenuation bands occurring after fabrication, as the hydrogen diffuses out of the fibre . LPGs fabricated in hydrogen-loaded fibre by irradiation at 193 nm have been observed to exhibit a growth in the peak loss of up to 14 dB and an increase in central wavelength of 40 nm over the first 20 h following UV exposure, followed by a slow reduction of the peak loss and decrease in central wavelength of 50 nm over the following 450 h . The effect is attributed to depletion of hydrogen in the exposed regions of the core. The diffusion of hydrogen from unexposed to exposed regions then acts to increase the amplitude of the refractive index modulation, as the refractive index increases further in the exposed regions (increasing hydrogen concentration) and decreases in the unexposed region (decreasing hydrogen concentration). Thus the strength of the LPG grows. This is followed by a slow outdiffusion whereby the refractive index of the core decreases, causing a decrease in wavelength. Similar effects have been observed for LPGs fabricated in hydrogen-loaded fibres using 248 nm irradiation . These effects limit the ability to fabricate LPGs with precisely defined characteristics within hydrogen-loaded fibre. It has been shown that pre-exposure of a hydrogen-loaded fibre to a uniform UV beam locks in the photosensitivity enhancement provided by the hydrogen loading procedure . The UV pre-exposure of the hydrogenloaded fibre increases the number of defect sites believed to be responsible for photosensitivity, and these remain after the hydrogen has diffused out of the fibre. If an LPG is fabricated in pre-exposed fibre after the hydrogen has diffused out of the fibre, typically 2 weeks after removal from the hydrogen atmosphere at room temperature, the fibre maintains the photosensitivity, but does not suffer from the changes in attenuation band central wavelength and extinction . Such effects have been observed using continuous-wave (CW) pre-exposure at 244 nm  and using pulsed irradiation at 157 nm  and 193 nm. Post-fabrication tuning of the characteristics of an LPG’s transmission spectrum is possible by reducing the fibre diameter by etching. The reduction in cladding diameter changes the effective index of the cladding modes, resulting in an increase in the central wavelengths of the attenuation bands. The etching also changes the electric field profile of the cladding modes, resulting in a change in the overlap integral and a concomitant change in the coupling efficiency and minimum transmission of the attenuation bands [36, 37]. Other UV wavelengths are being investigated for LPG formation, including 157 nm from F2 lasers which offers the
Stretching and twisting point
Figure 4. Corrugated fibre LPG.
ability to fabricate LPGs in low-GeO2 fibre with no hydrogen pre-treatment —fibres in which LPGs would not form when exposed to other UV wavelengths. In addition, LPG formation in hydrogen-loaded fibres using this wavelength required a fluence 250 times lower than that required from a laser operating at 248 nm . The frequency-doubled (266 nm)  and -tripled (355 nm)  outputs of Nd:YAG lasers have also been used to fabricate LPGs, as have femtosecond pulses from an Nd:glass laser . LPGs have been fabricated using irradiation with femtosecond pulses in the near infrared (800 nm) . The irradiation is believed to cause a densification of the glass, and the resultant index change, and LPG spectrum, is stable at temperatures up to 500 ◦ C. CO2 laser irradiation at 10.6 µm has been shown to produce LPGs with high temperature stability and polarization insensitivity , and with spectral characteristics that are unchanged even after annealing at 1200 ◦ C . The CO2 laser exposure of the fibre was originally thought to result in the densification of the glass, and/or the relaxation of tensile stresses built into the cladding of fibres such as Corning SMF28 during fabrication . However, there is evidence to suggest that the change in refractive index is a result of breakage of Si–O–Ge chains . CO2 laser irradiation has allowed LPGs to be written in both fibres that have been hydrogen loaded and in fibres with no hydrogen pre-treatment. The LPGs fabricated in hydrogenloaded fibre were associated with few extraneous spectral features, as a result of the lower fluence required for their fabrication . Electric arc fabrication of an LPG relies upon a combination of up to four effects to generate the periodic modulation of the fibre properties. The mechanisms exploited include the induction of microbends into the fibre , the periodic tapering of the fibre , the diffusion of dopants [12, 13] and the relaxation of internal stresses . Such LPGs have been shown to operate at temperatures of up to 800 ◦ C without permanent modification of their properties , and, if annealed appropriately, they may operate at temperatures up to 1190 ◦ C . Typically, the electrodes of a fusion-splicing machine are used, exposing a region of fibre with a length of the order of 100 µm to the arc, limiting the minimum period of LPG that may be fabricated. Chemical etching of the cladding of a fibre to produce a corrugated structure has been shown to allow the generation of an LPG . The corrugated fibre is shown in figure 4. When a tensile load is applied to the fibre, the periodic variation in the diameter of the fibre results in a periodic strain variation across the corrugated structure, with a concomitant periodic refractive index induced via the photoelastic effect. R51
Review Article 900
1 2 3 4 5 6 7 8 9
LPG period (µm)
Thus the coupling strength increases with applied load, with a small change in wavelength of the attenuation bands . Generally, LPGs have been fabricated to operate at telecommunications wavelengths (1300 and 1550 nm), and the spectrum is monitored by coupling light from superfluorescent fibre sources or superluminescent diodes in the fibre and recording the transmission using an optical spectrum analyser. There have been reports of the use of fibres with lower cutoff wavelengths, 650 nm, allowing the operation of the LPG within the response of silicon detectors, facilitating the use of low-cost CCD spectrometers .
700 600 500 400 300 200
3. LPG theory
λ = [n e f f (λ) −
n iclad (λ)]
is satisfied , where n e f f (λ) is the effective refractive index of the propagating core mode at wavelength λ, n iclad (λ) is the refractive index of the i th cladding mode and is the period of the LPG. The minimum transmission of the attenuation bands is governed by the expression  Ti = 1 − sin2 (κi L)
where L is the length of the LPG and κi is the coupling coefficient for the i th cladding mode, which is determined by the overlap integral of the core and cladding mode and by the amplitude of the periodic modulation of the mode propagation constants. Since the cladding generally has a large radius, it supports a large number of cladding modes. Theoretical analysis has shown that efficient coupling is possible only between core and cladding modes that have a large overlap integral, i.e. modes that have similar electric field profiles . Thus coupling is observed between the core and circularly symmetric cladding modes of odd order. This is because the electric field profile of the even-order modes is such that the field amplitude is low within the core, whereas the electric field profiles of the odd modes have a peak located within the core . The modelling of LPGs requires the calculation of the refractive indices of the core and cladding modes to allow the central wavelengths of the attenuation bands to be determined, and the calculation of the mode electric field profiles to facilitate determination of the coupling strength and the form of the spectrum. The refractive index of the propagating core mode of the fibre is generally determined using the weakly guided field approximation of Gloge . A simple three-layer slab waveguide model to determine the cladding mode indices has been presented, allowing an approximate determination of the coupling wavelengths . However, it has been shown that the effect of the core upon the effective indices and mode profiles of the cladding mode cannot be ignored for accurate simulation of LPG characteristics . R52
LPG period (µm)
The fibre itself consists of two waveguide structures—one being the high-index core surrounded by the lower-index cladding, the other being the cladding, surrounded by air. Phase matching between the mode propagating in the core of the fibre and a forward-propagating cladding mode is achieved at the wavelength, λ, where the expression
20 21 22 23 24 25 26 27
90 80 70 60 50
Figure 5. Plot of resonant wavelength as a function of LPG period for coupling between the guided core mode and cladding modes of order (a) 1–9 and (b) 18–29, calculated using the technique detailed in the text and assuming the fibre’s cut-off wavelength is 650 nm.
Figure 5 shows the dependence of the coupling wavelength for cladding modes 1–9 (a) and 18–27 (b) upon the period of the LPG. These graphs were calculated following the method presented in . The fibre modelled has a cut-off wavelength of 675 nm. The graphs indicate that coupling to lower-order modes is achieved using longer periods, while shorter periods facilitate coupling to the higher-order modes. In addition, figure 5(b) shows that, for higher-order cladding modes, coupling to one cladding mode can occur at two wavelengths, producing two attenuation bands . It should be noted that small changes in the coupling conditions could result in large changes in the separation of the two attenuation bands. For LPGs fabricated such that their period coincides with the peak of the curve (for example, mode 18), it has been observed that changes in the coupling conditions result in a change in the coupling efficiency, but not in the wavelength .
4. LPG sensors 4.1. Temperature sensitivity As discussed in the introduction, the sensitivity of LPGs to environmental parameters is influenced by the period of the LPG , by the order of the cladding mode to which coupling takes place  and by the composition of the optical fibre . This combination of influences allows the fabrication of LPGs that have a range of responses to a particular measurand—a single LPG may have attenuation bands that have a positive sensitivity to a measurand, others that are insensitive to the measurand and others with a negative sensitivity.
This property has been widely exploited for controlling the temperature sensitivity of LPGs. For many telecommunications applications spectral stability is of prime importance, and the ability to fabricate an LPG with an inherently temperatureinsensitive attenuation band is an attractive feature. This is also attractive for forming temperature-insensitive strain sensors. On the other hand, for forming temperature sensors, or thermally tuned filters, a high temperature sensitivity (of either sign) is required. The origin of the temperature sensitivity may be understood by differentiating equation (1) . dn e f f dλ 1 dL dλ dn cl dλ + = − (3) dT d(δn e f f ) dT dT d L dT where λ is the central wavelength of the attenuation band, T is the temperature, n e f f is the effective refractive index of the core mode, n cl is the effective refractive index of the cladding mode, δn e f f = (n e f f − n cl ), L is the length of the LPG and is the period of the LPG. The first term on the right-hand side of equation (3) is the material contribution, and is related to the change in the differential refractive index of the core and cladding arising from the thermo-optic effect. This contribution is dependent upon the composition of the fibre and is strongly dependent upon the order of the cladding mode. For coupling to loworder cladding modes (accessed using longer periods, > 100 µm), the material effect dominates. For coupling to higher-order cladding modes (accessed using shorter periods, < 100 µm), the material effect for standard germanosilicate fibres can be negligible . The second term is the waveguide contribution as it results from changes in the LPG’s period. The magnitude and sign of the term depend upon the order of the cladding mode. For coupling to low-order cladding modes dλ/d is positive, while for the higher-order cladding modes this term is negative, as can be seen from the graphs in figures 5(a) and (b). Thus, by an appropriate choice of LPG period it is possible to balance the two contributions to the temperature sensitivity to produce a temperature-independent attenuation band and also to produce attenuation bands with temperature sensitivities (positive or negative) appropriate to specific applications. Altering the fibre composition, such that the thermo-optic coefficient of the core is either larger or smaller than that of the cladding, can also be used to obtain a required temperature sensitivity . In addition to the change in central wavelength, a change in the extinction of the attenuation band may be observed for LPGs with strength κ L > π . At room temperature, the temperature response of the wavelengths of the attenuation bands’ is linear, as illustrated in figure 6 . However, it has been shown that the response becomes non-linear at cryogenic temperatures, below 77 K . LPGs fabricated in standard telecommunications optical fibre exhibit temperature sensitivities in the range 3 nm/100 ◦ C to 10 nm/100 ◦ C . This is an order of magnitude larger than the sensitivity of FBG sensors. Temperature-compensated LPGs have been demonstrated using periods 100 µm, the material contribution is negative, while the waveguide contribution is positive. Appropriate choice of grating period and fibre composition will thus allow the generation of attenuation bands with positive, negative or zero sensitivity to strain . An LPG of period 340 µm, written in Corning Flexcore fibre, exhibited an attenuation band with strain sensitivity of 0.04 pm µε−1 , which is an order of magnitude less than that of a FBG operating at 1300 nm. An LPG with period of 40 µm exhibited a larger strain sensitivity of −2.2 pm µε−1 , since in this regime, < 100 µm, both contributions to the strain sensitivity are negative . A typical response to strain is shown in figure 7, in which the wavelength shifts in the central wavelengths of a number of the attenuation bands of an LPG of period 280 µm, written in Corning SMF 28 fibre, are plotted as a function of strain . Each attenuation band exhibits a different, linear, response to the applied strain. The ability to define the performance of an LPG by virtue of its periodicity, making the LPG (i) strain insensitive ( > 100 µm) and (ii) temperature insensitive ( < 100 µm), offers a convenient method for isolating the response of the LPG to one or other of the measurands, since the periodicities correspond to the regimes in which the LPG can show (i) the highest sensitivity to temperature and (ii) the highest sensitivity to strain. The dependence of the sensitivity of the LPG to strain and temperature upon the order of the cladding mode R54
Figure 7. Shift in the wavelengths of four attenuation bands, A–D, as a function of strain for the LPG detailed in figure 6(a). The dashed line is the strain-induced wavelength shift for an FBG fabricated at 1550 nm for comparison. (From .)
may also be used to permit the decoupling of the temperature and strain responses, while simultaneously measuring both parameters , which has long been an issue in fibre optic sensing schemes. In addition to the measurement of axial strain, the sensitivity of LPGs to transverse loads has been investigated [63, 64]. The application of a transverse load induces linear birefringence in the optical fibre, with the result that each attenuation band is split into two, the bands corresponding to the two orthogonal polarization states, as shown in figure 8. Since the wavelengths of the two components are related to the birefringence, the wavelength separation increases with applied load. A linear response was obtained, with a sensitivity of 500 nm kg−1 mm−1 , which is 800 times that of a FBG . Corrugated LPGs have been used to form axial strain sensors and torsion sensors . As discussed in the fabrication section, the application of axial load to a fibre that has a periodically modified diameter results in the fibre experiencing a periodic strain, which, via the photoelastic effect, causes a periodic modulation of the refractive index of the fibre. The effect of axial load is thus to increase the coupling strength of the LPG, changing the minimum transmission of the LPG attenuation bands. A corrugated fibre experiencing torsion sees different twisting rates in the etched and unetched regions as a result of the difference in diameter. This results in a stress concentration at the etched boundary. The effect of torsion is to both change the coupling strength, and induce a wavelength shift [65, 66]. 4.3. Refractive index sensitivity The refractive index sensitivity of LPGs arises from the dependence of the phase matching condition upon the effective refractive index of the cladding modes. The effective indices of the cladding modes are dependent upon the difference between the refractive index of the cladding and that of the medium surrounding the cladding. The central wavelengths of the attenuation bands thus show a dependence upon the refractive
Figure 8. Loading system and transmission spectra of an LPG of period 490 µm, written in B–Ge co-doped fibre, unloaded and loaded, showing the generation of attenuation band splitting resulting from the induced birefringence. (After .) 5
(a) Wavelength Shift (nm)
0 -5 -10 -15 -20 -25 -30
1.38 1.40 1.42 1.44 1.46 1.48 1.50 1.52 1.54 1.56 1.58 1.60 1.62
-10 -15 -20 -25 -30 -35 1.38 1.40 1.42 1.44 1.46 1.48 1.50 1.52 1.54 1.56 1.58 1.60 1.62
Figure 9. Plot of (a) the wavelength shift and (b) the minimum transmission value of an attenuation band against the RI of the material surrounding the LPG of period 400 µm written in boron–germanium co-doped fibre with cut off wavelength 650 nm. (From .)
index of the medium surrounding the cladding, provided that the cladding has the higher refractive index. The sensitivity to refractive index manifests itself as a change in the central wavelengths and in the minimum transmission value of the attenuation bands, as is illustrated
in figure 9(a). The highest sensitivity is shown by the higherorder modes, and occurs at refractive indices approaching that of the cladding . When the refractive index is equal to that of the cladding, the cladding appears to be of infinite extent and thus supports no discrete modes. Broadband radiation-mode coupling losses are then observed, with no distinct attenuation bands. For surrounding refractive indices higher than that of the cladding, the centre wavelengths of the attenuation bands show a considerably reduced sensitivity [67–69], but a change in the form of the transmission spectrum is observed, in that the extinction of the attenuation bands is reduced , as is illustrated in figure 9(b). The presence of attenuation bands in this situation, where the cladding is no longer acting as a waveguide, is attributed to the existence of attenuated cladding modes arising from Fresnel reflection, rather than total internal reflection from the cladding/air interface . Clearly, for some applications where well-controlled spectral characteristics are required, the refractive index sensitivity has a number of practical implications for the packaging and protection of an LPG. Care has to be taken to ensure that the properties of an adhesive used to attach an LPG to a substrate, or the properties of materials used to protect the LPG from mechanical damage or humidity, do not change the wavelengths of the attenuation bands from their original value, and that any changes in the refractive index of the surrounding material do not cause a change in the transmission spectrum of the LPG. With this in mind, LPGs have been fabricated in fibres with complex structures to desensitize the LPG spectrum to the surrounding refractive index. LPGs fabricated in dual shaped core (DSC) dispersion-shifted fibre exhibit an attenuation band that is insensitive to external refractive index and to mechanical damage of the fibre surface . The DSC fibre contains an inner cladding region that has a higher refractive index than the remaining cladding layer. The refractive-index-insensitive attenuation band is believed to correspond to coupling to a mode of this inner cladding. LPGs have been fabricated in an air-clad optical fibre, in which the cladding of the fibre is surrounded by a capillary tube, supported by thin silica webs . The evanescent R55
Wavelength Shift (nm)
field of the cladding modes does not extend beyond the capillary, with the result that all of the attenuation bands are insensitive to the external refractive index. A similar fibre structure, but in which the space between the capillary and the inner cladding is filled with a liquid crystal material, has been used to create a tuneable filter. In this case, the refractive index of a dye doped nematic liquid crystal was controlled by realignment of the molecules using polarized laser illumination . Similar systems could be controlled using electrical or thermal techniques. The refractive index sensitivity of LPGs has been exploited to form refractive index sensors, chemical concentration sensors [74–76], a liquid level sensor  and as a means of forming a tuneable spectral filter . While LPGs are sensitive over only a limited refractive index range, and their response is not species specific, it has been shown that LPGs may be used for on-line monitoring of the concentration of aqueous solutions of materials or of materials in inaccessible locations for industrial production quality control . Concentrations of solutions of sodium chloride , calcium chloride  and ethylene glycol [67, 76] have been measured, with sensitivities equal to, or better than, that of conventional Abbe refractometry . The use of LPGs to monitor the refining of kerosene, which requires that the concentration of organic aromatics such as benzene and xylene is measured, has been proposed. To demonstrate the feasibility, the concentration of a binary solution of xylene in heptane was measured with a minimum detectable volumetric concentration of 0.04%, corresponding to a refractive index change of This is comparable to the accuracy 6 × 10−5 . of the standard technique of liquid chromatography and UV spectroscopy. The use of two cascaded LPGs, with periods chosen such that one LPG had an attenuation band that was insensitive to temperature while the other had a band that was insensitive to refractive index, has been shown to allow simultaneous, independent measurement of these two parameters. This potentially allows the temperature-independent monitoring of chemical solutions with temperature-dependent refractive indices . The majority of studies to date have concentrated upon the bulk immersion of the LPG into a solution. It is attractive to consider the prospect of depositing overlay materials that exhibit changes in their refractive index in response to their local environment. In this way, the LPG may be used to form, for example, a tuneable loss filter , a temperatureinsensitive filter  or a species-specific chemical sensor . LPG-based biosensors have been investigated by immobilizing antibodies on the surface of the fibre and monitoring the change in refractive index that occurs when an antigen bonds with the antibody . This is the first reported example of the use of an LPG to form a species-specific chemical sensor, again offering comparable performance to other techniques including surface plasmon resonance and interferometry, but with the prospect for on-line monitoring. The effect of the thickness of the overlay material upon the LPG response has also been investigated . A thin film of organic material was deposited upon an LPG using the Langmuir–Blodgett technique, which allows high-resolution control (≈3 nm) over the thickness of the film by depositing one molecular layer at a time. It was observed that, for
5 0 -5
200 400 600 Overlay Thickness (nm)
Figure 10. Experimentally determined response of two of the attenuation bands of an LPG to the deposition of a thin film of material of refractive index 1.57. (From .)
films of refractive index higher than that of the cladding, the wavelength and amplitudes of the attenuation bands exhibited a very high sensitivity to the optical thickness of the overlay when the thickness of the films was of the order of a few hundred nanometres. For materials of index lower than that of the cladding, the sensitivity to thickness of the overlay is considerably reduced. This is quite distinct from the behaviour under bulk immersion, in which the highest sensitivity is observed for indices lower than that of the cladding, as shown in figure 9(a). An example of this response is shown in figure 10. Materials suitable for deposition by the LB technique have been previously shown to be chemically sensitive [81, 82], offering the prospect for the development of a range of new species-specific chemical sensors. The refractive index sensitivity of LPGs has been exploited to form other types of physical sensor. LPGs have been proposed to form a flow sensor to monitor the arrival of resin within a liquid composite moulding system [83, 84]. The measurement relies upon the reduction in the extinction ratio of the attenuation band that occurs when the LPG is surrounded by a material of higher refractive index. An LPG-based liquid-level sensor has been reported . Partial immersion of the LPG within a liquid results in each attenuation band splitting into two. One of the split attenuation bands has a central wavelength corresponding to coupling to the cladding mode with an air surround (B), while the other has a central wavelength corresponding to coupling to the same cladding mode, but with its effective refractive index modified by having the liquid surround (A), as illustrated in figure 11. As the minimum transmission value of an attenuation band is dependent on the length of the LPG (according to equation (2)) then the relative depth of the split attenuation bands will change in response to a change in the liquid level. The sensor has a linear response, as shown in figure 12. The refractive index sensitivity has also been used to enhance and reduce the temperature sensitivity of LPGs. Surrounding the LPG by a liquid with a large thermo-optic coefficient results in the LPG responding to both changes in temperature and to the temperature-induced refractive index change of the surrounding medium [54–56]. If the material has a negative thermal expansion coefficient then, for increasing temperature, the wavelength shift induced by the change in refractive index of the coating causes a red shift in the wavelength of the attenuation band. If the attenuation band itself has positive temperature sensitivity, then the two
B λ (nair) wavelength
Figure 11. Principle of operation of the liquid-level sensor: (a) deployment of the LPG; (b) schematic of the expected split in the attenuation band. Relative change in transmission (%) 160 140 120 100 80 60 40
Ultra high sensitivity of up to 1900 nm/100 ◦ C, over a limited temperature range of 1 ◦ C, has been obtained by surrounding the fibre with a Cargille oil of refractive index that was approximately equal to that of the cladding. The sensor could be designed to operate at a range of temperatures by choosing an oil whose thermo-optic coefficient was such that, at the required operating temperature, the refractive index was approximately equal to that of the cladding . 4.4. Bend sensitivity
20 0 -20
5 10 15 20 25 30 35 40 45 50 55 60 65 70 75 80 85 90 95 100
% of LPG immersed in oil
Figure 12. Relative change in the extinction of the attenuation bands of the liquid-level sensors, exhibiting a linear response over 60% of the LPG’s length. (From .)
effects add to increase the temperature response. If, however the material has a positive thermo-optic coefficient, then an increase in temperature causes a blue shift of the attenuation band, reducing the temperature response of the attenuation band. Recoating the LPG with a UV-curable acrylate-based polymer of refractive index approximately equal to that of the cladding, and with a negative thermo-optic coefficient, increased the sensitivity of an LPG fabricated in a conventional dispersion-shifted fibre from 5 nm/100 ◦ C to 80 nm/100 ◦ C . This, however, was accompanied by a change in the coupling strength. Using an air-clad optical fibre, described previously in this section, in which the air regions were filled by the same polymer, produced a similar sensitivity but with no change in the minimum transmission of the attenuation bands . In addition, it was noted that the novel fibre structure allowed the polymer to be protected from environmental effects, such as humidity, that may degrade its performance. A similar system using a liquid crystal material produced a sensitivity of 210 nm/100 ◦ C . For an LPG recoated with a material of positive thermo-optic coefficient, a temperature response as low as 0.07 nm/100 ◦ C was obtained .
The bend sensitivity of an LPG manifests itself in one of two ways: as a shift in the central wavelength of the attenuation bands or as a splitting in two of each attenuation band, with the wavelength separation of the split components increasing with increasing curvature. The first observation of the influence of bending upon the transmission spectrum of an LPG noted that the shift in the central wavelength of the attenuation bands was accompanied by a reduction in the loss and a broadening of the spectral dropout . The magnitude of the bend-induced wavelength shift was subsequently observed to depend upon the orientation of the optical fibre with respect to the plane in which the bend is applied, with the maximum and minimum sensitivities separated by 180◦ . The origin of the orientation dependence is believed to be an eccentricity of the fibre core, with the core no longer at the neutral axis of the fibre. Fibres with eccentricities of up to 14 µm have been used to form bipolar bend sensors . The second manifestation—the splitting of the attenuation bands—is attributed to a breaking of the symmetry of the system that results in two degenerate spatial modes of the cladding becoming non-degenerate. The effect on the spectrum is shown in figure 13. This effect has been observed in B–Ge co-doped photosensitive fibre [39, 88] and in fibres with large core eccentricities . This effect also has been observed to exhibit a dependence upon the orientation of the fibre [39, 89]. In this case the reference plane is defined by the orientation of the fibre during fabrication of the LPG, with the largest sensitivity corresponding to the surface of the fibre oriented towards the UV source on the outer surface of the bend . This is thought to be a result of an asymmetry R57
Figure 15. Principle of operation of in-series LPGs. (From .)
1000 1010 1020 1030 1040 1050 1060 1070
Wavelength (nm) Figure 13. A plot of the transmission spectrum of an attenuation band in the spectrum of an LPG experiencing different bend curvatures. Solid curve, curvature 0.00 m−1 ; dashed curve, curvature 1.55 m−1 . The LPG of period 400 µm and length 40 mm was fabricated in B–Ge co-doped optical fibre with cut-off wavelength 650 nm. (From .)
Figure 14. Transmission spectrum of a pair of in-series LPGs: (a) with a 50 mm spacing; (b) with a 190 mm spacing. (From .)
introduced by a radially non-symmetric UV-induced refractive index modulation. Such asymmetries have been used to account for similar effects in LPGs formed by CO2 laser irradiation, where the asymmetry is more pronounced due to heating of the surface facing the laser beam . As discussed in the theory section, for higher-order cladding modes it is possible to couple to the same cladding mode at two different wavelengths. The wavelength separation of the two resulting attenuation bands shows high sensitivity to external measurands, and has been exploited to perform bend sensing, offering sensitivities of up to 50 times that offered by the previously reported LPG bend sensors . 4.5. In-series LPGs There has been some interest in the use of concatenated LPGs for sensing applications. When a pair of identical LPGs is fabricated in series within an optical fibre, separated by up to 10 cm, a set of fringes are observed within the attenuation bands, as seen in figure 14. The formation of the fringes may be understood with reference to figure 15. The first LPG couples light to the cladding mode. Light then propagates to the second LPG via two routes: in the core and in the cladding. R58
By virtue of the difference in the effective refractive indices of the core and cladding modes, the light coupled into the core by the second LPG is phase shifted with respect to the light propagating in the core, giving rise to the interference pattern. The narrower bandwidth of the fringe facilitates greater resolution in the measurement of the wavelength than is possible with conventional LPGs. In-series LPGs have been used to sense bending , external index of refraction [92, 93], temperature and transverse load . Bending the fibre results in an increase in the attenuation of the cladding modes, with a concomitant reduction in the fringe visibility, along with a shift in the central wavelength of the band . Transverse loading was observed to reduce the fringe visibility linearly until, at a threshold load, the fringe pattern disappeared . Further increase of the load causes the pattern to reappear with a π phase shift . The response of the in-series LPGs to refractive index is a decrease in fringe visibility and a change in the central wavelengths, of similar form to that observed for single LPGs . For refractive indices higher than that of the cladding, the fringes reappear, but with considerably reduced visibility. If, however, only the section of fibre between the LPGs is surrounded by the material of high refractive index, the minimum transmission of the attenuation bands can show up to twice the sensitivity of a conventional LPG, for refractive indices in the range 1.5– 1.55 . Coating the end of a fibre containing an LPG with a metal film results in the double pass of the light through the LPG, allowing the generation of the interference fringes characteristic of in-series LPGs . This also allows the monitoring of the performance of the LPG in reflection, and avoids the need to fabricate identical LPGs. This has been used to form a temperature sensor . 4.6. Multi-parameter sensing using LPGs As has been discussed previously, the sensitivity of LPGs to the various measurands is dependent on the composition of the fibre, the period of the LPG and the order of the cladding mode to which coupling takes place. Appropriate choice of fibre composition and grating period allows the generation of attenuation bands that are insensitive to temperature or strain, facilitating independent measurement of these measurands . Alternatively, the differential shifts in two or more resonance bands of a single LPG may be used to measure simultaneously and independently the temperature and strain, by virtue of the difference in their sensitivities to the measurands . The observation of the bendinduced splitting of the attenuation bands has allowed the simultaneous measurement of bend radius and temperature, where the wavelength separation of the split components of the attenuation band gave a measurement of bend radius, while the average wavelength was dependent upon temperature . LPGs have been used in conjunction with FBGs to separate their temperature and strain responses , and also
to demodulate the return from the FBG . Two FBGs were fabricated such that their Bragg wavelengths sat on either side of the spectrum of an attenuation band of an LPG physically located on the source side of the two FBGs. Thus the LPG acted to attenuate the reflections from the FBGs, the attenuation being dependent upon their relative central wavelengths. By virtue of the difference between the sensitivities of the FBGs and LPGs to strain and temperature, a small decrease in the measured reflection of the low-wavelength FBG, accompanied by a small increase in the reflection from the higher-wavelength FBG, indicated a change in strain, while a large increase in the reflection from the low-wavelength FBG, accompanied by a large decrease in the reflection from the longer-wavelength FBG indicated a change in temperature. Measurement of the relative intensities of the reflections allowed independent measurement of temperature and strain . An LPG was also used as an edge filter to facilitate an intensity based method to demodulate the reflection from an FBG .
5. Summary The sensitivity of LPGs to strain, temperature, bending and external refractive index, the ability to tune the sensitivity by virtue of fibre composition and LPG period, and the presence of features with the transmission spectrum that show differing sensitivities to the various measurands offer the prospect for the development of sensor elements capable of simultaneously and independently monitoring a number of measurands. This paper has discussed the properties of LPGs, techniques for their fabrication and the origin of their sensitivity to the various measurands. The means for optimizing the performance of the LPG for particular applications has been outlined, along with a review of the uses to which they have been put.
Acknowledgments The authors would like to acknowledge the support of the Engineering and Physical Sciences Research Council, UK and the Royal Society.
References  Kashyap R 1999 Fibre Bragg Gratings (New York: Academic)  Kersey A D, Davis M A, Patrick H J, LeBlanc M, Koo K P, Askins C G, Putnam M A and Friebele E J 1997 Fiber grating sensors J. Lightwave Technol. 15 1442–63  Bhatia V 1999 Applications of long-period gratings to single and multi-parameter sensing Opt. Express 4 457–66  Bhatia V and Vengsarkar A M 1996 Optical fibre long-period grating sensors Opt. Lett. 21 692–4  Chen K P, Herman P R, Tam R and Zhang J 2000 Rapid long-period grating formation in hydrogen loaded fibre with 157 nm F2 laser radiation Electron. Lett. 36 2000–1  Guan B-Ou, Tam H-Y, Ho S-L, Liu S-Y and Dong X-Y 2000 Growth of long-period gratings in H2 -loaded fibre after 193 nm UV inscription IEEE Photon. Technol. Lett. 12 642–4  Blows J and Tang D Y 2000 Gratings written with tripled output of Q-switched Nd:YAG laser Electron. Lett. 36 1837–9  Fujumaki M, Ohki Y, Brebner J L and Roorda S 2000 Fabrication of long-period optical fibre gratings by use of ion implantation Opt. Lett. 25 88–90
 Kondo Y, Nouchi K, Mitsuyu T, Watanabe M, Kazansky P and Hirao K 1999 Fabrication of long-period fibre gratings by focused irradiation of infra-red femtosecond laser pulses Opt. Lett. 24 646–8  Davis D D, Gaylord T K, Glytsis E N, Kosinski S G, Mettler S C and Vengsarkar A M 1998 Long-period fibre grating fabrication with focused CO2 laser beams Electron. Lett. 34 302–3  Drozin L, Fonjallaz P-Y and Stensland L K 2000 Long-period fibre gratings written by CO2 exposure of H2 -loaded standard fibres Electron. Lett. 36 742–3  Dianov E M, Karpov V I, Grekov M V, Golant K M, Vasiliev S A, Medvekov O I and Khrapko R R 1997 Thermo-induced long period fibre grating IOOC-ECOC 1997 vol 2 (London: IEE) pp 53–6  Dianov E M, Karpov V I, Kurkov A S and Grekov M V 1998 Long period fibre gratings and mode-field converters fabricated by thermodiffusion in phosphosilicate fibres 24th ECOC vols 1–3 (Madrid: Telefonica Espana) pp 395–6  Kim C S, Han Y, Lee B H, Han W-T, Paek U-C and Chung Y 2000 Induction of the refractive index change in B-doped optical fibers through relaxation of the mechanical stress Opt. Commun. 185 337–42  Rego G, Okhotnikov O, Dianov E and Sulimov V 2001 High-temperature stability of long-period fibre gratings using an electric arc J. Lightwave Technol. 19 1574–9  Palai P, Satyanarayan M N, Das M, Thyagarajan K and Pal B P 2001 Characterisation and simulation of long period gratings fabricated using electric discharge Opt. Commun. 193 181–5  Savin S, Digonnet M J F, Kino G S and Shaw H J 2000 Tunable mechanically induced long-period fibre gratings Opt. Lett. 25 710–12  Jiang Y, Li Q, Lin C H, Lyons E, Tomov I and Lee H P 2002 A novel strain-induced thermally tuned long-period fibre grating fabricated on a periodic corrugated silicon fixture IEEE Photon. Technol. Lett. 14 941–3  Kakarantzas G, Dimmick T E, Birks T A, Le Roux R and Russell P St J 2001 Miniature all-fibre devices based on CO2 microstructuring of tapered fibres Opt. Lett. 26 1137–9  Poole C D, Presby H M and Meester J P 1994 Two mode fibre spatial-mode converter using periodic core deformation Electron. Lett. 30 1437–8  Narayanan C, Presby H M and Vengsarkar A M 1996 Band-rejection fibre filter using periodic core deformation OFC 1996 (San Jose, USA) pp 267–8  Lin C-Y, Chern G-W and Wang L A 2001 Periodical corrugated structure for forming sampled fibre Bragg grating and long-period fibre grating with tunable coupling strength J. Lightwave Technol. 19 1212–20  Kakarantzas G, Birks T A and Russell P S 2002 Structural long-period gratings in photonic crystal fibers Opt. Lett. 27 1013–15  Kashyap R 1999 Fibre Bragg Gratings (London: Academic)  Williams D L, Ainslie B J, Armitage J R, Kashyap R and Campbell R 1993 Enhanced UV photosensitivity in boron codoped germanosilicate fibers Electron. Lett. 29 45–7  Lemaire P J, Atkins R M, Mizrahiu V and Reed W A 1993 High pressure H2 -loading as a technique for achieving ultrahigh UV photosensitivity and thermal sensitivity in GeO2 doped optical fibers Electron. Lett. 29 1191–3  Vengsarkar A M, Lemaire P J, Judkins J B, Bhatia V, Erdogan T and Sipe J E 1996 Long-period fibre gratings as band rejection filters J. Lightwave Technol. 14 58–64  Patrick H J, Askins C G, Mcelhanon R W and Friebele E J 1997 Amplitude mask patterned on an excimer laser mirror for high intensity writing of long period fibre gratings Electron. Lett. 33 1167–8  Lu S Y, Tan H Y and Demokan M S 1999 Low-cost microlens array for long-period grating fabrication Electron. Lett. 35 79–80  Private Communication, Oxford Lasers, UK
 Bennion I, Williams J A R, Zhang L, Sugden K and Doran N 1996 UV-written in-fibre Bragg gratings Opt. Quantum Electron. 28 93–135  Duhem O and Douay M 2000 Effect of UV-induced birefringence on long-period grating coupling characteristics Electron. Lett. 36 416–17  Jang J N, Kim H G, Shin S G, Kim M S, Lee S B and Kwack K H 1999 Effects of hydrogen molecule diffusion on LP0m mode coupling of long-period gratings J. Non-Cryst. Solids 259 156–64  Kawano H, Muentz H, Sato Y, Nishimae J and Sugitatsu A 2001 Reduction of transmission spectrum shift of long period fibre gratings by a UV-preexposure method J. Lightwave Technol. 19 1221–8  Chen K P, Wei X and Herman P R 2002 Strong 157 nm F2 -laser photosensitivity locking of hydrogen loaded telecommunication fibre for 248 nm fabrication of long-period gratings Electron. Lett. 38 17–18  Vasiliev S A, Dianov E M, Varelas D, Limberger H G and Salathe R P 1996 Post-fabrication resonance peak positioning of long period cladding-mode-coupled gratings Opt. Lett. 21 1830–2  Zhou K, Liu H and HU X 2001 Tuning the resonant wavelength of long period fibre gratings by etching the fibre’s cladding Opt. Commun. 197 295–9  Chen K P, Herman P R, Zhang J and Tam R 2001 Fabrication of strong long-period gratings in hydrogen free fibers with 157 nm F2 -laser radiation Opt. Lett. 26 771–3  Ye C C, James S W and Tatam R P 2000 Simultaneous temperature and bend sensing using long-period fibre gratings Opt. Lett. 25 1007–9  Dragomir A, Nikogosyan D N, Ruth A A, Zagorul’ko K A and Kryukov P G 2002 Long-period fibre grating formation with 264 nm femtosecond radiation Electron. Lett. 38 269–71  Davis D D, Gaylord T K, Glytsis E N and Mettler S C 1998 CO2 laser induced long-period fibre gratings: spectral characteristic, cladding modes and polarisation independence Electron. Lett. 34 1416–17  Hwang I K, Yun S H and Kim B Y 1999 Long period fibre grating based upon periodic microbends Opt. Lett. 24 1263–5  Humbert G and Malki A 2002 Electric-arc-induced gratings in non-hydrogenated fibres: fabrication and high-temperature characterizations J. Opt. A: Pure Appl. Opt. 4 194–8  Bhatia V, Campbell D K, Sherr D, D’Alberto T G, Zabaronick N A, Ten Eyck G A, Murphy K A and Claus R O 1997 Temperature-insensitive and strain insensitive long-period grating sensors for smart structures Opt. Eng. 36 1872–6  Erdogan T 1997 Cladding mode resonances in short and long period fibre grating filters J. Opt. Soc. Am. 14 1760–73 Erdogan T 2000 Cladding mode resonances in short and long period fibre grating filters: errata J. Opt. Soc. Am. 17 2113  Gloge D 1971 Weakly guiding fibres Appl. Opt. 10 2252–8  Patrick H J, Kersey A D and Bucholtz F 1998 Analysis of the response of long period fibre gratings to external index of refraction J. Lightwave Technol. 16 1606–42  Han Y G, Lee B H, Han W T, Paek U C and Chung Y 2001 Resonance peak shift and dual peak separation of long period fibre gratings for sensing applications IEEE Photon. Technol. Lett. 13 699–701  Grubsky V and Feinberg J 2000 Long period fibre gratings with variable coupling for real-time sensing applications Opt. Lett. 25 203–5  Shima K, Himeno K, Sakai T, Okude S and Wada A 1997 A novel temperature-insensitive long-period grating using a boron-codoped germanosilicate core-fibre Tech. Dig. OFC’97 pp 347–8  Ng M N and Chiang K S 2002 Thermal effects on the transmission spectra of long-period fiber gratings Opt. Commun. 208 321–7
 James S W, Tatam R P, Bateman R, Twin A and Noonan P 2003 Cryogenic temperature response of fibre optic long period gratings Electron. Lett. submitted  Shu X, Allsop T, Gwandu B, Zhang L and Bennion I 2001 High temperature sensitivity of long-period gratings in B–Ge codoped fibre IEEE Photon. Technol. Lett. 13 818–20  Yin S, Chung K-W and Zhu X 2001 A highly sensitivity long period grating based tuneable filter using a unique double cladding layer structure Opt. Commun. 188 301  Khaliq S, James S W and Tatam R P 2002 Enhanced sensitivity fibre optic long period grating temperature sensor Meas. Sci. Technol. 13 792–5  Abramov A A, Hale A, Windeler R S and Strasser T A 1999 Widely tunable long-period fibre gratings Electron. Lett. 35 81–2  Qin L, Wei Z X, Wang Q Y, Li H P, Zheng W, Zhang Y S and Gao D S 2000 Compact temperature compensating package for long period fibre gratings Opt. Met. 14 239–42  Jang J N, Kim S Y, Kim S W and Kim M S 1999 Temperature insensitive long-period fibre gratings Electron. Lett. 35 2134  Ng M N, Chen Z H and Chiang K S 2002 Temperature compensation of long-period fiber grating for refractive-index sensing with bending effect IEEE Photon. Technol. Lett. 14 361–2  Duhem O, CaCosta A, Henninot J F and Douay M 1999 Long period copper coated grating as an electrically tuneable wavelength selective filter Electron. Lett. 35 1014–15  Constantini D M, Muller C A P, Vasiliev S A, Limberger H G and Salathe R P 1999 Tunable loss filter based on metal coated long-period fibre grating IEEE Photon. Technol. Lett. 11 1458–60  Bhatia V, Campbell D, Claus R O and Vengsarkar A M 1997 Simultaneous strain and temperature measurement with long-period gratings Opt. Lett. 22 648–50  Liu Y, Zhang L and Bennion I 1999 Fibre optic load sensors with high transverse strain sensitivity based on long-period gratings in B/Ge co-doped fibre Electron. Lett. 35 661–2  Zhang L, Liu Y, Williams J A R and Bennion I 1999 Design and realisation of long-period grating devices in conventional and high birefringence fibers and their novel applications as fibre optic load sensors IEEE J. Sel. Top. Quantum Electron. 5 1371–8  Lin C-Y, Wang L A and Chern G-W 2001 Corrugated long-period fibre gratings as strain, torsion and bending sensors J. Lightwave Technol. 19 1159–68  Wang L A, Lin C Y and Chern G W 2001 A torsion sensor made of a corrugated long period fibre grating Meas. Sci. Technol. 12 793–9  Patrick H J, Kersey A D and Bucholtz F 1998 Analysis of the response of long period fibre gratings to external index of refraction J. Lightwave Technol. 16 1606–42  Hou R, Ghassemlooy Z, Hassan A, Lu C and Dowker K P 2001 Modelling of long-period fibre grating response to refractive index higher than that of cladding Meas. Sci. Technol. 12 1709–13  Lee B H, Liu Y, Lee S B, Choi S S and Jang J N 1997 Displacements of the resonant peaks of a long-period fibre grating induced by a change of ambient refractive index Opt. Lett. 22 1769–71  Duhem O, Henninot J-F, Warenghem M and Douay M 1998 Demonstration of long-period grating efficient couplings with an external medium of a refractive index higher than that of silica Appl. Opt. 37 7223–8  Lee B H and Nishii J 1998 Cladding surrounding interface insensitive long-period grating Electron. Lett. 34 1129–30  Espindola R P, Windeler R S, Abramov A A, Eggerton B J, Strasser T A and DiGiovanni D J 1999 External refractive index insensitive air-clad long period fibre grating Electron. Lett. 35 327–8
 Yin S, Chung K-W and Zhu X 2001 A novel all-optic tuneable long period grating using a unique double cladding layer Opt. Commun. 196 181–6  Shu X and Huang D 1999 Highly sensitive chemical sensor based on the measurement of the separation of dual resonant peaks in a 100 µm period fibre grating Opt. Commun. 171 65–9  Allsop T, Zhang L and Bennion I 2001 Detection of organic aromatic compounds by a long period fibre grating optical sensor with optimised sensitivity Opt. Commun. 191 181–90  Falciai R, Mignani A G and Vannini A 2001 Long period gratings as solution concentration sensors Sensors Actuators B 74 74–7  Khaliq S, James S W and Tatam R P 2001 Fibre-optic liquid level sensor using a long-period grating Opt. Lett. 26 1224–6  Gwandu B A L, Shu X, Allsop T D P, Zhang W, Zhang L and Bennion I 2002 Simultaneous refractive index and temperature measurement using cascaded long-period grating in double-cladding fibre Electron. Lett. 38 695–6  DeLisa M P, Zhang Z, Shiloach M, Pilevar S, Davis C C, Sirkis J S and Bentley W E 2000 Evanescent wave long period fiber Bragg grating as an immobilized antibody biosensor Anal. Chem. 72 2895–900  James S W, Rees N D, Ashwell G J and Tatam R P 2002 Optical fibre long period gratings with Langmuir Blodgett thin film overlays Opt. Lett. 9 686–8  Flannery D, James S W, Tatam R P and Ashwell G J 1997 A pH sensor using Langmuir–Blodgett overlays on polished optical fibres Opt. Lett. 22 567–9  Flannery D, James S W, Tatam R P and Ashwell G J 1999 Fibre optic chemical sensing using Langmuir–Blodgett overlay waveguides Appl. Opt. 38 7370–4  Dankers J P, Lenhart J L, Kueh S R, van Zanten J H, Advani S G and Parnas R S 2001 Fibre optic flow and cure sensing for liquid composite molding Opt. Lasers Eng. 35 91–104  Kueh S R M, Parnas R S and Advani S G 2002 A methodology for using long-period gratings and mold-filling simulations to minimize the intrusiveness of flow sensors in liquid composite molding Compos. Sci. Technol. 62 311–27
 Xu M G, Maaskant R, Ohn M M and Alavie A T 1997 Independent tuning of cascaded long period fibre gratings for spectral shaping Electron. Lett. 33 1893–4  Patrick H J, Chang C C and Vohra S T 1998 Long period fibre gratings for structural bend sensing Electron. Lett. 18 1773–4  Patrick H J 2000 Self-aligning bipolar bend transducer based on long period grating written in eccentric core fibre Electron. Lett. 36 1763–4  Liu Y, Zhang L, Williams J A R and Bennion I 2000 Optical bend sensor based on measurement of resonance mode splitting of long-period fibre grating IEEE Photon. Technol. Lett. 12 531–3  Rathje J, Kristensen M and Hubner J 2000 Effects of fiber core concentricity error and UV illumination direction on the bend direction asymmetry of long-period gratings Bragg Gratings, Photosensitivity and Poling in Glass Waveguides (OSA Trends in Optics and Photonics vol 33) ed T Erodogan, E J Friebele and R Kashyap pp 210–28  VanWiggeren G D, Gaylord T K, Davies D D, Anemogiannis E, Garrett B D, Braiwish M I and Glytsis E N 2000 Axial rotation dependence of resonances in curved CO2 laser induced long-period fibre gratings Electron. Lett. 36 1354–5  Lee B H and Nishii J 1998 Bending sensitivity of in-series long period fibre gratings Opt. Lett. 23 1624–6  Duhem O, Henninot J F and Douay M 2000 Study of a fibre Mach–Zehnder interferometer based on two spaced 3 dB long period gratings surrounded by a refractive index higher than that of silica Opt. Commun. 180 225–62  Han Y G, Lee B H, Han W T, Paek U C and Chung Y 2001 Fibre optic sensing applications of a pair of long period fibre gratings Meas. Sci. Technol. 12 778–81  Lee B H and Nishii J 1998 Self-interference of long-period fibre grating and its application as temperature sensor Electron. Lett. 34 2059–60  Patrick H J, Williams G M, Kersey A D, Pedrazzani J R and Vengsarkar A M 1996 Hybrid fibre Bragg grating/long period grating sensor for strain/temperature discrimination IEEE Photon. Technol. Lett. 8 1223–5  Fallon R W, Zhang L, Williams J A R and Bennion I 1998 All-fibre optical sensing system: Bragg grating sensor interrogated by a long period grating Meas. Sci. Technol. 9 1969–73